#------------------------------------------------------------------------------
#$Date: 2021-04-30 11:19:27 +0300 (Fri, 30 Apr 2021) $
#$Revision: 264720 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/23/1562310.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562310
loop_
_publ_author_name
'Li, Na'
'Mu, Bao'
'Cao, Xinyu'
'Huang, Rudan'
_publ_section_title
;
 The structures and properties of the new two-dimensional
 inorganic--organic hybrid materials based on the molybdate chains
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              180
_journal_page_last               186
_journal_paper_doi               10.1016/j.jssc.2014.06.001
_journal_volume                  217
_journal_year                    2014
_chemical_formula_sum            'C16 H18 Mn Mo6 N6 O22'
_chemical_formula_weight         1276.94
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                106.443(2)
_cell_angle_beta                 91.5990(10)
_cell_angle_gamma                98.7530(10)
_cell_formula_units_Z            1
_cell_length_a                   7.6364(5)
_cell_length_b                   10.1462(7)
_cell_length_c                   10.3819(8)
_cell_measurement_reflns_used    2046
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      28.418
_cell_measurement_theta_min      3.149
_cell_volume                     760.37(9)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.980
_diffrn_measured_fraction_theta_max 0.980
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0229
_diffrn_reflns_av_sigmaI/netI    0.0511
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            3821
_diffrn_reflns_theta_full        25.02
_diffrn_reflns_theta_max         25.02
_diffrn_reflns_theta_min         3.15
_exptl_absorpt_coefficient_mu    2.900
_exptl_absorpt_correction_T_max  0.7043
_exptl_absorpt_correction_T_min  0.3901
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_density_diffrn    2.789
_exptl_crystal_density_meas      0
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             609
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.13
_refine_diff_density_max         1.240
_refine_diff_density_min         -1.196
_refine_diff_density_rms         0.212
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.034
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     232
_refine_ls_number_reflns         2621
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.034
_refine_ls_R_factor_all          0.0521
_refine_ls_R_factor_gt           0.0388
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0680P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1036
_refine_ls_wR_factor_ref         0.1129
_reflns_number_gt                2061
_reflns_number_total             2621
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2014-217-180.cif
_cod_data_source_block           5
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Triclinic' was changed to
'triclinic' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               1562310
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.70134(9) 0.30751(7) 0.86389(6) 0.0130(2) Uani 1 1 d . . .
Mo2 Mo 0.99865(8) 0.58931(6) 0.87919(6) 0.01148(19) Uani 1 1 d . . .
Mo3 Mo 0.49902(8) 0.57445(7) 0.86322(6) 0.0131(2) Uani 1 1 d . . .
Mn1 Mn 1.0000 0.5000 0.5000 0.0188(4) Uani 1 2 d S . .
N1 N 0.8867(10) 0.7485(7) 0.4045(7) 0.0255(17) Uani 1 1 d . . .
N2 N 0.9046(10) 0.7072(7) 0.5152(7) 0.0260(17) Uani 1 1 d . . .
N3 N 0.6907(9) 1.0615(7) 0.1431(7) 0.0255(17) Uani 1 1 d . . .
H3 H 0.6645 1.1015 0.0840 0.031 Uiso 1 1 calc R . .
O1 O 0.7488(7) 0.5366(5) 0.8791(5) 0.0171(12) Uani 1 1 d . . .
O2 O 0.9582(6) 0.3752(5) 0.9078(5) 0.0127(11) Uani 1 1 d . . .
O3 O 0.4840(7) 0.3751(5) 0.9107(5) 0.0147(11) Uani 1 1 d . . .
O4 O 0.6909(7) 0.2651(6) 0.6912(5) 0.0226(13) Uani 1 1 d . . .
O5 O 0.7399(7) 0.4107(5) 1.0882(5) 0.0162(11) Uani 1 1 d . . .
O6 O 0.6739(8) 0.1501(6) 0.8983(6) 0.0252(13) Uani 1 1 d . . .
O7 O 1.0195(7) 0.5207(6) 0.7074(5) 0.0228(13) Uani 1 1 d . . .
O8 O 0.9982(7) 0.7611(6) 0.8999(5) 0.0223(13) Uani 1 1 d . . .
O9 O 0.5756(7) 0.7435(6) 0.8721(6) 0.0254(13) Uani 1 1 d . . .
O10 O 0.4501(7) 0.4942(6) 0.6946(5) 0.0256(14) Uani 1 1 d . . .
O11 O 0.7227(7) 0.4023(6) 0.4907(6) 0.0305(15) Uani 1 1 d . . .
H11B H 0.6504 0.4470 0.4644 0.037 Uiso 1 1 d R . .
H11C H 0.6934 0.3868 0.5641 0.037 Uiso 1 1 d R . .
C1 C 0.8386(13) 0.7969(9) 0.6134(9) 0.031(2) Uani 1 1 d . . .
H1 H 0.8321 0.7916 0.7012 0.038 Uiso 1 1 calc R . .
C2 C 0.7817(12) 0.8979(9) 0.5676(9) 0.031(2) Uani 1 1 d . . .
H2 H 0.7332 0.9735 0.6174 0.037 Uiso 1 1 calc R . .
C3 C 0.8105(11) 0.8655(8) 0.4342(9) 0.0243(19) Uani 1 1 d . . .
C4 C 0.6403(13) 1.1074(9) 0.2666(9) 0.034(2) Uani 1 1 d . . .
H4 H 0.5773 1.1813 0.2883 0.040 Uiso 1 1 calc R . .
C5 C 0.6817(12) 1.0451(9) 0.3629(9) 0.028(2) Uani 1 1 d . . .
H5 H 0.6496 1.0786 0.4505 0.033 Uiso 1 1 calc R . .
C6 C 0.7704(12) 0.9335(8) 0.3295(8) 0.0236(19) Uani 1 1 d . . .
C7 C 0.8220(12) 0.8898(9) 0.1992(9) 0.029(2) Uani 1 1 d . . .
H7 H 0.8846 0.8158 0.1746 0.034 Uiso 1 1 calc R . .
C8 C 0.7810(12) 0.9552(8) 0.1068(9) 0.026(2) Uani 1 1 d . . .
H8 H 0.8156 0.9261 0.0195 0.031 Uiso 1 1 calc R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O6 Mo1 O4 104.6(3) . .
O6 Mo1 O3 103.8(2) . .
O4 Mo1 O3 104.3(2) . .
O6 Mo1 O2 102.4(2) . .
O4 Mo1 O2 100.7(2) . .
O3 Mo1 O2 137.5(2) . .
O6 Mo1 O1 164.7(2) . .
O4 Mo1 O1 90.6(2) . .
O3 Mo1 O1 72.9(2) . .
O2 Mo1 O1 72.94(19) . .
O6 Mo1 O5 87.6(2) . .
O4 Mo1 O5 167.3(2) . .
O3 Mo1 O5 75.22(19) . .
O2 Mo1 O5 73.08(18) . .
O1 Mo1 O5 77.04(19) . .
O8 Mo2 O7 104.1(3) . .
O8 Mo2 O1 96.7(2) . .
O7 Mo2 O1 98.4(2) . .
O8 Mo2 O5 100.8(2) . 2_767
O7 Mo2 O5 88.5(2) . 2_767
O1 Mo2 O5 159.0(2) . 2_767
O8 Mo2 O2 91.6(2) . 2_767
O7 Mo2 O2 159.1(2) . 2_767
O1 Mo2 O2 93.3(2) . 2_767
O5 Mo2 O2 74.78(19) 2_767 2_767
O8 Mo2 O2 163.1(2) . .
O7 Mo2 O2 91.5(2) . .
O1 Mo2 O2 74.3(2) . .
O5 Mo2 O2 85.73(19) 2_767 .
O2 Mo2 O2 75.0(2) 2_767 .
O9 Mo3 O10 104.0(3) . .
O9 Mo3 O5 99.7(2) . 2_667
O10 Mo3 O5 97.6(2) . 2_667
O9 Mo3 O1 91.2(2) . .
O10 Mo3 O1 98.9(2) . .
O5 Mo3 O1 157.5(2) 2_667 .
O9 Mo3 O3 158.1(2) . .
O10 Mo3 O3 92.9(2) . .
O5 Mo3 O3 91.5(2) 2_667 .
O1 Mo3 O3 72.4(2) . .
O9 Mo3 O3 91.5(2) . 2_667
O10 Mo3 O3 163.9(2) . 2_667
O5 Mo3 O3 75.2(2) 2_667 2_667
O1 Mo3 O3 84.90(19) . 2_667
O3 Mo3 O3 73.2(2) . 2_667
O7 Mn1 O7 180.000(1) . 2_766
O7 Mn1 O11 91.2(2) . 2_766
O7 Mn1 O11 88.8(2) 2_766 2_766
O7 Mn1 O11 88.8(2) . .
O7 Mn1 O11 91.2(2) 2_766 .
O11 Mn1 O11 180.0(3) 2_766 .
O7 Mn1 N2 82.8(2) . 2_766
O7 Mn1 N2 97.2(2) 2_766 2_766
O11 Mn1 N2 88.6(2) 2_766 2_766
O11 Mn1 N2 91.4(2) . 2_766
O7 Mn1 N2 97.2(2) . .
O7 Mn1 N2 82.8(2) 2_766 .
O11 Mn1 N2 91.4(2) 2_766 .
O11 Mn1 N2 88.6(2) . .
N2 Mn1 N2 180.000(2) 2_766 .
N2 N1 C3 109.7(7) . .
C1 N2 N1 106.6(7) . .
C1 N2 Mn1 133.0(6) . .
N1 N2 Mn1 119.9(5) . .
C4 N3 C8 122.4(7) . .
C4 N3 H3 118.8 . .
C8 N3 H3 118.8 . .
Mo2 O1 Mo3 151.2(3) . .
Mo2 O1 Mo1 106.2(2) . .
Mo3 O1 Mo1 101.8(2) . .
Mo1 O2 Mo2 105.9(2) . 2_767
Mo1 O2 Mo2 104.0(2) . .
Mo2 O2 Mo2 105.0(2) 2_767 .
Mo1 O3 Mo3 107.2(2) . .
Mo1 O3 Mo3 103.0(2) . 2_667
Mo3 O3 Mo3 106.8(2) . 2_667
Mo3 O5 Mo2 156.1(3) 2_667 2_767
Mo3 O5 Mo1 102.6(2) 2_667 .
Mo2 O5 Mo1 100.4(2) 2_767 .
Mo2 O7 Mn1 159.1(3) . .
Mn1 O11 H11B 113.0 . .
Mn1 O11 H11C 113.0 . .
H11B O11 H11C 110.5 . .
N2 C1 C2 110.6(8) . .
N2 C1 H1 124.7 . .
C2 C1 H1 124.7 . .
C3 C2 C1 106.0(7) . .
C3 C2 H2 127.0 . .
C1 C2 H2 127.0 . .
N1 C3 C2 107.1(7) . .
N1 C3 C6 121.7(7) . .
C2 C3 C6 131.2(7) . .
N3 C4 C5 119.7(8) . .
N3 C4 H4 120.2 . .
C5 C4 H4 120.2 . .
C6 C5 C4 120.0(8) . .
C6 C5 H5 120.0 . .
C4 C5 H5 120.0 . .
C5 C6 C7 118.3(7) . .
C5 C6 C3 119.2(8) . .
C7 C6 C3 122.5(7) . .
C8 C7 C6 120.2(8) . .
C8 C7 H7 119.9 . .
C6 C7 H7 119.9 . .
N3 C8 C7 119.5(8) . .
N3 C8 H8 120.3 . .
C7 C8 H8 120.3 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O6 1.717(5) .
Mo1 O4 1.718(5) .
Mo1 O3 1.914(5) .
Mo1 O2 1.973(5) .
Mo1 O1 2.256(5) .
Mo1 O5 2.257(5) .
Mo2 O8 1.695(5) .
Mo2 O7 1.743(5) .
Mo2 O1 1.901(5) .
Mo2 O5 2.016(5) 2_767
Mo2 O2 2.145(5) 2_767
Mo2 O2 2.251(5) .
Mo3 O9 1.702(6) .
Mo3 O10 1.712(5) .
Mo3 O5 1.923(5) 2_667
Mo3 O1 2.014(5) .
Mo3 O3 2.201(5) .
Mo3 O3 2.252(5) 2_667
Mn1 O7 2.102(5) .
Mn1 O7 2.102(5) 2_766
Mn1 O11 2.185(6) 2_766
Mn1 O11 2.185(6) .
Mn1 N2 2.294(7) 2_766
Mn1 N2 2.294(7) .
N1 N2 1.340(9) .
N1 C3 1.362(10) .
N2 C1 1.328(11) .
N3 C4 1.324(11) .
N3 C8 1.338(10) .
N3 H3 0.8600 .
O2 Mo2 2.145(5) 2_767
O3 Mo3 2.252(5) 2_667
O5 Mo3 1.923(5) 2_667
O5 Mo2 2.016(5) 2_767
O11 H11B 0.8500 .
O11 H11C 0.8500 .
C1 C2 1.366(12) .
C1 H1 0.9300 .
C2 C3 1.363(12) .
C2 H2 0.9300 .
C3 C6 1.490(11) .
C4 C5 1.379(12) .
C4 H4 0.9300 .
C5 C6 1.373(11) .
C5 H5 0.9300 .
C6 C7 1.388(12) .
C7 C8 1.365(11) .
C7 H7 0.9300 .
C8 H8 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
C3 N1 N2 C1 0.6(10) . . . .
C3 N1 N2 Mn1 173.3(5) . . . .
O7 Mn1 N2 C1 -15.2(9) . . . .
O7 Mn1 N2 C1 164.8(9) 2_766 . . .
O11 Mn1 N2 C1 -106.6(9) 2_766 . . .
O11 Mn1 N2 C1 73.4(9) . . . .
N2 Mn1 N2 C1 102(100) 2_766 . . .
O7 Mn1 N2 N1 174.3(6) . . . .
O7 Mn1 N2 N1 -5.7(6) 2_766 . . .
O11 Mn1 N2 N1 82.9(6) 2_766 . . .
O11 Mn1 N2 N1 -97.1(6) . . . .
N2 Mn1 N2 N1 -69(100) 2_766 . . .
O8 Mo2 O1 Mo3 16.4(6) . . . .
O7 Mo2 O1 Mo3 -89.0(6) . . . .
O5 Mo2 O1 Mo3 162.8(5) 2_767 . . .
O2 Mo2 O1 Mo3 108.3(6) 2_767 . . .
O2 Mo2 O1 Mo3 -178.2(6) . . . .
O8 Mo2 O1 Mo1 -177.0(2) . . . .
O7 Mo2 O1 Mo1 77.7(3) . . . .
O5 Mo2 O1 Mo1 -30.5(7) 2_767 . . .
O2 Mo2 O1 Mo1 -85.0(2) 2_767 . . .
O2 Mo2 O1 Mo1 -11.54(18) . . . .
O9 Mo3 O1 Mo2 -11.3(6) . . . .
O10 Mo3 O1 Mo2 93.1(6) . . . .
O5 Mo3 O1 Mo2 -130.5(6) 2_667 . . .
O3 Mo3 O1 Mo2 -176.6(6) . . . .
O3 Mo3 O1 Mo2 -102.7(6) 2_667 . . .
O9 Mo3 O1 Mo1 -178.2(2) . . . .
O10 Mo3 O1 Mo1 -73.8(3) . . . .
O5 Mo3 O1 Mo1 62.6(6) 2_667 . . .
O3 Mo3 O1 Mo1 16.44(18) . . . .
O3 Mo3 O1 Mo1 90.4(2) 2_667 . . .
O6 Mo1 O1 Mo2 87.7(9) . . . .
O4 Mo1 O1 Mo2 -87.7(3) . . . .
O3 Mo1 O1 Mo2 167.6(3) . . . .
O2 Mo1 O1 Mo2 13.3(2) . . . .
O5 Mo1 O1 Mo2 89.3(2) . . . .
O6 Mo1 O1 Mo3 -98.9(9) . . . .
O4 Mo1 O1 Mo3 85.8(3) . . . .
O3 Mo1 O1 Mo3 -18.9(2) . . . .
O2 Mo1 O1 Mo3 -173.2(3) . . . .
O5 Mo1 O1 Mo3 -97.2(2) . . . .
O6 Mo1 O2 Mo2 -65.6(3) . . . 2_767
O4 Mo1 O2 Mo2 -173.4(2) . . . 2_767
O3 Mo1 O2 Mo2 61.4(4) . . . 2_767
O1 Mo1 O2 Mo2 99.2(2) . . . 2_767
O5 Mo1 O2 Mo2 17.97(19) . . . 2_767
O6 Mo1 O2 Mo2 -176.0(2) . . . .
O4 Mo1 O2 Mo2 76.3(3) . . . .
O3 Mo1 O2 Mo2 -48.9(4) . . . .
O1 Mo1 O2 Mo2 -11.07(18) . . . .
O5 Mo1 O2 Mo2 -92.3(2) . . . .
O8 Mo2 O2 Mo1 72.5(8) . . . .
O7 Mo2 O2 Mo1 -85.2(2) . . . .
O1 Mo2 O2 Mo1 13.1(2) . . . .
O5 Mo2 O2 Mo1 -173.6(2) 2_767 . . .
O2 Mo2 O2 Mo1 111.0(3) 2_767 . . .
O8 Mo2 O2 Mo2 -38.4(8) . . . 2_767
O7 Mo2 O2 Mo2 163.8(2) . . . 2_767
O1 Mo2 O2 Mo2 -97.9(2) . . . 2_767
O5 Mo2 O2 Mo2 75.4(2) 2_767 . . 2_767
O2 Mo2 O2 Mo2 0.0 2_767 . . 2_767
O6 Mo1 O3 Mo3 -177.8(2) . . . .
O4 Mo1 O3 Mo3 -68.5(3) . . . .
O2 Mo1 O3 Mo3 55.6(4) . . . .
O1 Mo1 O3 Mo3 17.72(19) . . . .
O5 Mo1 O3 Mo3 98.4(2) . . . .
O6 Mo1 O3 Mo3 69.7(3) . . . 2_667
O4 Mo1 O3 Mo3 179.0(2) . . . 2_667
O2 Mo1 O3 Mo3 -56.9(4) . . . 2_667
O1 Mo1 O3 Mo3 -94.8(2) . . . 2_667
O5 Mo1 O3 Mo3 -14.07(18) . . . 2_667
O9 Mo3 O3 Mo1 -62.7(7) . . . .
O10 Mo3 O3 Mo1 78.4(3) . . . .
O5 Mo3 O3 Mo1 176.1(2) 2_667 . . .
O1 Mo3 O3 Mo1 -20.0(2) . . . .
O3 Mo3 O3 Mo1 -109.9(3) 2_667 . . .
O9 Mo3 O3 Mo3 47.2(7) . . . 2_667
O10 Mo3 O3 Mo3 -171.7(3) . . . 2_667
O5 Mo3 O3 Mo3 -74.0(2) 2_667 . . 2_667
O1 Mo3 O3 Mo3 89.9(2) . . . 2_667
O3 Mo3 O3 Mo3 0.0 2_667 . . 2_667
O6 Mo1 O5 Mo3 -88.5(3) . . . 2_667
O4 Mo1 O5 Mo3 105.8(10) . . . 2_667
O3 Mo1 O5 Mo3 16.5(2) . . . 2_667
O2 Mo1 O5 Mo3 167.8(3) . . . 2_667
O1 Mo1 O5 Mo3 92.0(2) . . . 2_667
O6 Mo1 O5 Mo2 85.0(3) . . . 2_767
O4 Mo1 O5 Mo2 -80.7(10) . . . 2_767
O3 Mo1 O5 Mo2 -170.0(3) . . . 2_767
O2 Mo1 O5 Mo2 -18.7(2) . . . 2_767
O1 Mo1 O5 Mo2 -94.6(2) . . . 2_767
O8 Mo2 O7 Mn1 -26.9(10) . . . .
O1 Mo2 O7 Mn1 72.2(9) . . . .
O5 Mo2 O7 Mn1 -127.7(9) 2_767 . . .
O2 Mo2 O7 Mn1 -164.3(6) 2_767 . . .
O2 Mo2 O7 Mn1 146.6(9) . . . .
O7 Mn1 O7 Mo2 -15(100) 2_766 . . .
O11 Mn1 O7 Mo2 99.6(9) 2_766 . . .
O11 Mn1 O7 Mo2 -80.4(9) . . . .
N2 Mn1 O7 Mo2 -172.0(9) 2_766 . . .
N2 Mn1 O7 Mo2 8.0(9) . . . .
N1 N2 C1 C2 -1.4(11) . . . .
Mn1 N2 C1 C2 -172.8(6) . . . .
N2 C1 C2 C3 1.6(12) . . . .
N2 N1 C3 C2 0.4(10) . . . .
N2 N1 C3 C6 -178.6(7) . . . .
C1 C2 C3 N1 -1.2(11) . . . .
C1 C2 C3 C6 177.7(9) . . . .
C8 N3 C4 C5 0.3(14) . . . .
N3 C4 C5 C6 -1.8(15) . . . .
C4 C5 C6 C7 2.4(14) . . . .
C4 C5 C6 C3 -178.7(8) . . . .
N1 C3 C6 C5 175.2(8) . . . .
C2 C3 C6 C5 -3.6(15) . . . .
N1 C3 C6 C7 -5.9(13) . . . .
C2 C3 C6 C7 175.3(10) . . . .
C5 C6 C7 C8 -1.4(13) . . . .
C3 C6 C7 C8 179.6(8) . . . .
C4 N3 C8 C7 0.7(13) . . . .
C6 C7 C8 N3 -0.1(13) . . . .
